Synthesis, characterization and electrocatalytic activity of silver
nanorods towards the reduction of benzyl chloride
T. Maiyalagan *
Department of Chemistry, School of Science and Humanities, VIT University, Vellore 632014, India
Received 3 October 2007; received in revised form 9 February 2008; accepted 13 February 2008
Available online 17 February 2008
This paper describes a simple method of synthesizing silver nanorods using the polyol process, where propylene glycol serves both as a reducing
agent and as a solvent in the presence of a capping reagent such as polyvinylpyrrolidone (PVP). The diameter and length of silver nanorods could be
controlled by changing the AgNO3/PVP ratio. The end-to-end assembly of the silver nanorods was found. The silver nanorods were characterized by
using scanning electron microscopy, transmission electron microscopy, X-ray diffraction and absorption spectroscopy. The catalytic activity of a
glassy carbon electrode with Ag nanorods exhibits extraordinary electrocatalytic activities towards the electro-reduction of benzyl chloride.
# 2008 Elsevier B.V. All rights reserved.
Keywords: Silver nanorods; Polyol process; Reducing agent; Capping reagent; Electro-reduction
Nanomaterials of noble metals have received much attention
due to their potential application in microelectronics, optical
and catalytic properties [1–5]. The synthesis of metal
nanoparticles of desired size and shape has enormous
importance in nanotechnology because of their characteristic
shape and size dependent optical, electronic and chemical
properties. The novel properties of these materials have found
extensive uses in microelectronics, electronics, magnetic
devices, non-linear optics, chemical and biochemical sensors
and in catalysis [5–7]. Among the known nanoparticles, Ag is
widely studied because of its characteristic optical, spectro-
scopic and catalytic properties. They have been widely
exploited for use in photography, catalysis, biological labeling,
photonics and surface enhanced Raman scattering, among
others. A rich variety of recipes are now available in the
literature for the synthesis of Ag nanoparticles. However, it has
been observed in most cases, that due to the existence of a
highly exposed surface, the nanoparticles tend to aggregate and
form large clusters even during the preparative process.
Therefore, a need to control the particle–particle interactions
so as to obtain a stable dispersion has been acutely felt by
researchers in this community. It is generally accepted that the
preparation of discrete silver nanoparticles with well-deﬁned
shape and well-controlled dimensions is more difﬁcult than
preparation of gold ones due to the higher reactivity of silver
compounds. Here we report the formation of silver nanorods,
through direct reduction of AgNO3 by the solvent (propylene
glycol) at 170 8C in the presence of a stabilizer polymer PVP.
By varying the concentration of silver salt and PVP as well as
the temperature, one can conveniently control the shape of the
resulting nanoparticles. These results are in agreement with
those reported by Xia and co-workers in a number of recent
papers using the polyol process [8–12]. It was shown that silver
nanorods formed in a modiﬁed polyol process as a result of the
aggregation of previously formed nanoparticles.
An exciting and hitherto unexploited silver nanorod has been
needed for electrode applications. Electrocatalytic reduction of
organic halides (RX) has been a central topic in organic
electrochemistry for the last few decades [13–17]. Among
various examined electrode materials, silver has been found to
possess extraordinary electrocatalytic properties [18–32].
In the present paper, we report a simple chemical synthesis
of silver nanorods. The as-prepared silver nanorods were
characterized by transmission electron microscopy (TEM),
scanning electron microscopy (SEM), powder X-ray diffraction
(XRD) and UV absorption spectrum measurements. The
Available online at www.sciencedirect.com
Applied Catalysis A: General 340 (2008) 191–195
* Tel.: +91 416 2202465; fax: +91 416 2243092.
E-mail address: firstname.lastname@example.org.
0926-860X/$ – see front matter # 2008 Elsevier B.V. All rights reserved.
electrochemical reduction of benzyl chloride is evaluated by
cyclic voltammetry and is interpreted in comparison with that
of conventional silver electrodes. Here we report the results of
an investigation on the potentialities of silver nanorods as an
electrocatalyst in the electro-reduction of benzyl chloride.
Poly (N-vinyl-2-pyrrolidone) (PVP, MW $ 40 000, supplied
by Fluka), silver nitrate (AgNO3) and the solvents used in the
study were analytical grade reagents and were used as received.
2.2. Synthesis of silver nanorods
The synthesis was performed within a three-neck round
beaker, which was heated in an oil bath up to 170 8C and then
10 ml of AgNO3 and 20 ml of PVP solution in glycol were
added in turn. The reﬂuxing was maintained for 90 min; small
aliquots were then withdrawn during the reaction for TEM. The
mixture was diluted with water and nanorods were collected by
2.3. Structural characterization
XRD patterns were obtained by a powder diffractometer
(XRD-SHIMADZU XD-D1) using a Ni-ﬁltered Cu Ka X-ray
radiation source. The morphology of the silver nanorods was
investigated by SEM (FEI, Model: Quanta 200). TEM, electron
diffraction and energy dispersive X-ray analysis (EDAX) were
performed on a Philips CM12/STEM instrument. For UV–vis
absorption investigation, a certain amount of the obtained Ag
nanorod powders was dispersed in ethanol and determined with
a TU-1201 model spectrophotometer.
2.4. Electrochemical characterization
A single glass compartment cell with three electrodes was
employed for the cyclic voltammetry studies. Pt wire and
Fig. 1. (a–c) TEM images of silver nanorods formation during the course of reaction.
T. Maiyalagan / Applied Catalysis A: General 340 (2008) 191–195192
saturated calomel electrode (SCE) were used as counter and
reference electrode, respectively. A 0.076-cm2
area of glassy
carbon (GC) or silver served as the working electrode.
All electrochemical measurements were performed using a
CHI660A potentiostat/galvanostat. The glassy carbon was ﬁrst
polished with alumina paste (procured from BAS, USA)
followed by ultrasonication in water for 5 min; it was then
polished with diamond paste (3 mm) and again ultrasonicated
for 10 min in water. The nanorods was coated on a glassy
carbon electrode using naﬁon as the binder and dried in an oven
at 80 8C for 2 min to get a thin ﬁlm on glassy carbon electrode.
The electrolyte was degassed with nitrogen gas before the
3. Results and discussion
The formation of nanorods of silver can be visually observed
through a continuous color change from pale yellow during the
formation of initial seeds in the solution upon addition of
AgNO3 solution through red and green towards gray, as the
particles grow. A general observation in our TEM studies was
the presence of stripes made of small dots in the early stages of
the reaction, in contrast with long continuous rods when the
solution was allowed to boil for 90 min. Typical images are
shown in Fig. 1. It is clear that initially only small spherical dots
of nanoparticles exist (Fig. 1a); as the reaction proceeded
Fig. 2. Scanning electron microscope picture of silver nanorods.
Fig. 3. (a) EDX spectra (b) electron diffraction pattern and (c) XRD pattern of silver nanorods (X-ray source: Cu Ka radiation (l = 1.5418 A˚ ).
T. Maiyalagan / Applied Catalysis A: General 340 (2008) 191–195 193
further stripes (Fig. 1b) of various lengths and thickness for. As
the reaction proceeds, well-deﬁned rods are eventually obtained
(Fig. 1c). SEM (Fig. 2) results also show the well-deﬁned rods
The energy-dispersive X-ray analysis (Fig. 3a) of a sample
provides further evidence that the product is silver. Fig. 3b
displays the electron diffraction pattern formed by directing an
electron beam onto the silver nanorods. The pattern shows that
the silver nanorod tends to growth as a bicrystalline twinned
structure. On the basis of these ﬁndings, it is concluded that
nanorods consist of crystalline silver.
The structure of as-prepared silver nanorods was investi-
gated by XRD analysis. A typical XRD pattern of the silver
nanorods synthesized using the polyol process was found to
possess a face centered cubic structure (fcc) as shown in Fig. 3c.
Four distinct diffraction peaks were observed at 2u values of
38.18, 44.38, 64.48and 77.38, respectively, corresponding to the
(1 1 1), (2 0 0), (2 2 0) and (3 1 1) crystalline planes of cubic
Ag (JCPDS cards 4-0783). The result was similar to that
reported . The broad nature of the XRD peaks could be
attributed to the nano-size of the particles (Fig. 3c).
It is very interesting to investigate the optical properties of
silver since it absorbs strongly in the visible region due to
surface plasmon resonance [34,35]. The position of the
plasmon absorption peak depends on the particle size and
shape [36–38]. The UV–vis spectra of the silver nanoparticles
and nanorods are shown in Fig. 4. The silver nanoparticles
display plasmon absorption in the visible region and usually
have an absorption maximum at 404 nm . The silver
nanorods showed two plasmon bands in the UV–vis
absorption spectrum one at 424 nm and the other at
wavelengths ranging from 500 to 680 nm depending on the
length of the nanorods. Silver nanorods display an absorption
maximum at 424 nm, which is red-shifted about 20 nm
compared to the silver nanoparticles . The bigger the
aspect ratio the more red shifted is the longitudinal plasmon
We investigated the electro-reduction of benzyl chloride at
silver and GC electrodes. Two types of silver electrode were
used: one made from the bulk metal and the other was made from
glassy carbon-modiﬁed Ag nanorods (denoted GC/Ag nanor-
ods). On all three electrodes, a single irreversible peak is
observed in cyclic voltammetry. Fig. 5 shows examples of cyclic
voltammograms obtained for the electro-reduction of benzyl
chloride at GC, Ag and GC/Ag nanorod electrodes. As shown in
Fig. 5, benzyl chloride exhibits a single irreversible reduction
peak at all electrodes. The voltammetric behaviour of benzyl
chloride at Ag is quite similar to that observed at GC except for
the remarkable positive shift of the peak. Such a positive shift is
indicative of the catalytic role of Ag in the electrode process .
The position of the peak, however, depends strongly on the
electrode material. A signiﬁcant positive shift was observed at
the silver nanorod electrodes. The data obtained at GC, Ag and
GC/Ag nanorod electrodes are collected in Table 1.
The most important result emerging from such studies is that
silver nanorods exhibits extraordinary electrocatalytic activities
towards the electro-reduction process, especially in the case of
benzyl chloride. There is more positive shift in the reduction
potential for glassy carbon modiﬁed Ag nanorods electrode
compared to that for a polycrystalline Ag electrode. The
extraordinary electrocatalytic effect of Ag nanorods is probably
relatedtothe diffusioncontrolledprocessoccurringatthe surface
of the nanorods and to the high afﬁnity of the Ag nanorods with
Fig. 4. UV–vis spectra of silver nanoparticles and nanorods.
Fig. 5. Cyclic voltammograms recorded at 0.2 V sÀ1
in CH3CN + 0.1 M
Et4NClO4 at (a) GC electrode (b) Ag electrode and (c) GC/Ag nanorod
Voltammetric data for the reduction of benzyl chlorides (3 mM) in
CH3CN + 0.1 M Et4NClO4 at v = 0.2 V sÀ1
(V) Current density
GC À2.14 2.2
Ag À1.77 3.7
GC/Ag nanorods À1.66 6.5
Applied potential (V vs. SCE).
T. Maiyalagan / Applied Catalysis A: General 340 (2008) 191–195194
In summary, we have shown that silver nanorods form in
glycol solution through aggregation of smaller, spheroidal
nanoparticles at high temperature during reduction of AgNO3 in
the presence of PVP, under appropriate experimental conditions.
It is found that the concentrations of both AgNO3 and PVP play
an important part in the formation of nanorods. In conclusion, Ag
nanorods have shown good catalytic properties in the electro-
reduction of benzyl chlorides. Although the catalytic properties
of Ag nanorods originate from its afﬁnity for the chloride ions,
the possibility of extraordinary electrocatalytic effect of Ag
nanorods is linked to the morphology of the nanorods.
 R.P. Andres, J.D. Bielefeld, J.I. Henderson, D.B. Janes, V.R. Kolagunta,
C.P. Kubiak, W.J. Mahoney, R.I. Osifchin, Science 273 (1996) 1690.
 A.P. Alivasators, Science 271 (1996) 933.
 M. Mofﬁt, A. Eisenberg, Chem. Mater. 7 (1995) 1178.
 M.A. El-Sayed, Acc. Chem. Res. 34 (2001) 257.
 M. Valden, X. Lai, D.W. Goodman, Science 281 (1998) 1647.
 C.J. Murphy, Science 298 (2002) 2139.
 P.V. Kamat, J. Phys. Chem. B 106 (2002) 7729.
 N.R. Jana, T.K. Sau, T. Pal, J. Phys. Chem. 103 (1999) 115.
 S.K. Ghosh, S. Kundu, M. Madal, T. Pal, Langmuir 18 (2002) 8756.
 Y. Sun, B. Gates, B. Mayers, Y. Xia, Nano Lett. 2 (2002) 165.
 Y. Sun, Y. Xia, Adv. Mater. 14 (2002) 833.
 Y. Sun, Y. Yin, B.T. Mayers, T. Herricks, Y. Xia, Chem. Mater. 14 (2002)
 J.-M. Save´ant, Adv. Phys. Org. Chem. 26 (1990) 1.
 O.R. Brown, H.R. Thrisk, B. Thornton, Electrochim. Acta 16 (1971) 495.
 D.D. Tanner, J.A. Plambeck, D.W. Reed, T.W. Mojelsky, J. Org. Chem. 45
 D.A. Koch, B.J. Henne, D.E. Bartak, J. Electrochem. Soc. 134 (1987)
 C.P. Andrieux, A. Le Gorande, J.-M. Sav´eant, J. Am. Chem. Soc. 114
 S. Rondinini, P.R. Mussini, V. Ferzetti, D. Monti, Electrochim. Acta 36
 S. Rondinini, P.R. Mussini, P. Muttini, G. Sello, Electrochim. Acta 46
 M. Benedetto, G. Miglierini, P.R. Mussini, F. Pelizzoni, S. Rondinini, G.
Sello, Carbohydr. Lett. 1 (1995) 321.
 S. Rondinini, P.R. Mussini, G. Sello, E. Vismara, J. Electrochem. Soc. 145
 M. Guerrini, P. Mussini, S. Rondinini, G. Torri, E. Vismara, Chem.
Commun. (1998) 1617.
 S. Rondinini, P.R. Mussini, G. Cantu, G. Sello, Phys. Chem. Chem. Phys. 1
 M. Fedurco, C.J. Sartoretti, J. Augustynski, Langmuir 17 (2001) 2380.
 S. Ardizzone, G. Cappelletti, P.R. Mussini, S. Rondinini, L.M. Doubova, J.
Electroanal. Chem. 532 (2002) 285.
 A.A. Isse, A. Gennaro, Chem. Commun. (2002) 2798.
 S. Ardizzone, G. Cappelletti, L.M. Doubova, P.R. Mussini, S.M. Passeri,
S. Rondinini, Electrochim. Acta 48 (2003) 3789.
 P.R. Mussini, S. Ardizzone, G. Cappelletti, L.M. Doubova, M. Longhi, S.
Rondinini, J. Electroanal. Chem. 552 (2003) 213.
 A. Gennaro, C.M. Sa´nchez-Sa´nchez, A.A. Isse, V. Montiel, Electrochem.
Commun. 6 (2004) 627.
 A.A. Isse, M.G. Ferlin, A. Gennaro, J. Electroanal. Chem. 581 (2005) 38.
 C. Bellomunno, D. Bonanomi, L. Falciola, M. Longhi, P.R. Mussini, L.M.
Doubova, G. Di Silvestro, Electrochim. Acta 50 (2005) 2331.
 A.A. Isse, L. Falciola, P.R. Mussini, A. Gennaro, Chem. Commun. (2006)
 J.J. Zhu, S.W. Liu, O. Palchik, Y. Koltypin, A. Gedanken, Langmuir 16
 S. Kapoor, Langmuir 14 (1998) 1021.
 P. Mulvaney, S. Underwood, Langmuir 10 (1994) 3427.
 K.L. Kelly, E. Coronado, L.L. Zhao, G.C. Schatz, J. Phys. Chem. B 107
 K.S. Lee, M.A. El-Sayed, J. Phys. Chem. B 110 (2006) 19220.
 T. Itakura, K. Torigoe, K. Esumi, Langmuir 11 (1995) 4129.
 S. Link, M.B. Mohamed, M.A. El-Sayed, J. Phys. Chem. B 103 (1999)
 N.R. Jana, L. Gearheart, C.J. Murphy, J. Phys. Chem. B 105 (2001)
 A.A. Isse, A. De Giusti, A. Gennaro, L. Falciola, P.R. Mussini, Electro-
chem. Commun. 8 (2006) 1707.
T. Maiyalagan / Applied Catalysis A: General 340 (2008) 191–195 195